- Nano Express
- Open Access
Anodization of nanoporous alumina on impurity-induced hemisphere curved surface of aluminum at room temperature
© Chung et al; licensee Springer. 2011
- Received: 27 September 2011
- Accepted: 16 November 2011
- Published: 16 November 2011
Nanoporous alumina which was produced by a conventional direct current anodization [DCA] process at low temperatures has received much attention in various applications such as nanomaterial synthesis, sensors, and photonics. In this article, we employed a newly developed hybrid pulse anodization [HPA] method to fabricate the nanoporous alumina on a flat and curved surface of an aluminum [Al] foil at room temperature [RT]. We fabricate the nanopores to grow on a hemisphere curved surface and characterize their behavior along the normal vectors of the hemisphere curve. In a conventional DCA approach, the structures of branched nanopores were grown on a photolithography-and-etched low-curvature curved surface with large interpore distances. However, a high-curvature hemisphere curved surface can be obtained by the HPA technique. Such a curved surface by HPA is intrinsically induced by the high-resistivity impurities in the aluminum foil and leads to branching and bending of nanopore growth via the electric field mechanism rather than the interpore distance in conventional approaches. It is noted that by the HPA technique, the Joule heat during the RT process has been significantly suppressed globally on the material, and nanopores have been grown along the normal vectors of a hemisphere curve. The curvature is much larger than that in other literatures due to different fabrication methods. In theory, the number of nanopores on the hemisphere surface is two times of the conventional flat plane, which is potentially useful for photocatalyst or other applications.
PACS: 81.05.Rm; 81.07.-b; 82.45.Cc.
- anodic aluminum oxide
- porous alumina
- nanoporous template
Anodic aluminum oxide [AAO] can be classified into two types of structure, namely the barrier type and the porous type of structure. The barrier type with a thin and compact-packed structure has been widely used in protection and dielectric capacitors , while the porous-type structure has received much attention since the characteristic of a high-ordered nanopore arrangement was discovered . Recently, many researches have been focused on the nanostructured materials due to some of their significant physical properties . Although several techniques like photolithography, etching, or gas phase synthesis can produce nanowires or nanotubes , a template-assisted growing approach of nanoporous AAO is considered as one of the most prominent methods due to the advantages of a controllable diameter, high aspect ratio, and economical way in producing. The AAO template has been used in various applications such as multiple quantum wells , photonic crystals , light-emitting diodes , humidity sensors , nanomaterial syntheses , and supercapacitors . Recently, a typical electrochemical method for producing AAO films was developed using a potentiostatic two-step anodization on costly high-purity (99.997%) Al films . Other approaches such as pulse anodization  or isotropic etching [12, 13] have been employed to fabricate three-dimensional nanostructures. Many conventional AAO templates were performed using direct current anodization [DCA] at a low temperature (0°C to 10°C) to avoid Joule-heat-dissolution effect at a relatively high room temperature. Also, AAO templates are preferred to grow on Al foil with a smooth surface in order to avoid the nonuniform electric field during the anodization process. Therefore, Al foil should be electropolished before anodization. However, porous alumina with forms of curved spheres has been reported in the anodization of Al films. Yin et al.  made nanopore patterns on a photolithography-and-wet-etched Al curved surface on a Si substrate by a conventional DCA method and discussed that the bending and branching features should be accounted for the interpore distance mechanism. In this article, we have synthesized AAO on a hemisphere curved surface using a hybrid pulse anodization [HPA] method [15, 16] on low-purity (99%) Al foils at room temperature [RT]. HPA possesses more advantages than the conventional DCA not only in curbing the Joule heat, but also in operating at a higher RT due to effective cooling [15, 17]. The high-curvature hemisphere surface was induced by the high-resistivity impurities in Al foil during the HPA process. It is noted that the defects and impurities in the low-purity Al foil can sometimes bring disturbing effects for locally enhancing oxidation and dissolution rates during the anodization process to produce a hemisphere curve on the Al foil surface after removal of the first-step AAO. The detailed growth behavior and mechanism of anodization on the hemisphere curves were further investigated. The branching and bending phenomena of nanopores reported here are shown to be deeply induced by electric fields rather than by the interpore distance mechanism .
The low-purity aluminum foil (99%, Alfa Aesar, Ward Hill, MA, USA) was used by our two-step HPA method. The plate was cut into a piece of 1.5 × 1.0 cm in size and then electropolished in a mixture of HClO4 and ethanol (1:4 in volumetric ratio) at 20 V for 30 s at RT. The two-step HPA is performed in a 0.5-M oxalic acid at RT. First of all, the applied hybrid pulse was constructed from a positive square wave followed by another negative square wave with the duty ratio of 1:1. The voltage of 40 V was applied on the positive pulse, while the negative voltage of -2 V was adopted for the negative pulse. The period of a hybrid pulse was 2 s (1 s:1 s). The formation of AAO was performed for 1 h by means of the potentiostat (5000, JIEHAN Technology Corporation, Taichung, Taiwan), and the three-electrode electrochemical cell with the platinum mesh acted as the counter electrode, the gold-coated silicon, as the working electrode, and Ag/AgCl, as the reference electrode. In order to further study the behavior of the anodization process, the real-time time-current curves were recorded. After the anodization, the specimens were immersed in 5 wt.% phosphoric acid at 50°C for 60 min in order to remove all porous alumina structures. The second anodization process was subsequently conducted by the same pulse condition as the first anodization. The morphology and pore characteristics of AAO films were examined using a high-resolution field emission scanning electron microscope [HR-FESEM] (JSM-7001, JEOL, Tokyo, Japan).
where r is the radius of the concave (hemisphere), d is the thickness of the porous alumina, and λ is the original interpore distance in the curved surface. If the interpore distance is increased two times larger than that of the original interpore distance in the claim of Yin et al. , the branch will occur immediately. In our case, in Figure 2, the original interpore distance λ is 80 nm, r is 500 nm, and d is 3,000 nm. So the estimated increased interpore distance D t is about 89 nm. Thus, the branch behavior may not have resulted from increasing interpore distances, but from electric field variations.
where L is the length of the central pore channel and r and λ are the same as in Equation 1. Therefore, the depth difference also depends on the length of the pore channels. On the other hand, the electrical field strength on the interface of Al and alumina is concerned with the curvature of locations. The strongest electric field occurs in the cusp between pores. In the anodization of the flat Al foil, the depth for each pore channel is equal, so the influence of the strongest electric field is not clear. In the anodization of the curved Al, this unbalanced strongest electric field and small resistance from other pore walls lead to the central pore branching. With more branches being formed, the growth of the other pores will bend towards the outer area, as shown in Figure 3b. Therefore, a bending situation is more evident at the outer region of the concave center in the impurity-induced hemisphere curve.
where q is the heat transfer rate, k is thermal conductivity of Al, A is area, and ,,and are the temperature gradients in x, y, and z directions, respectively. In this case, we can assume that the heat transfer rates are equal in three directions, so the heat-affected zone would be in a shape of a hemisphere due to the lower thermal conductivity of alumina, as shown in Figure 4a. The isothermal is along the surface of the hemisphere. Therefore, the formation and dissolution rate of porous alumina in the impurity-induced heat-affected zone are accelerated, as shown in Figure 4b. However, this difference is not observed in the porous alumina surface. It occurred only when all first-step porous aluminas are being removed completely. It is also seen that lots of hemisphere curves occur on the Al foil surface, as shown in Figure 4c. After the second anodization, porous aluminas are formed on the hemisphere curved surface along the normal vectors, as shown in Figure 4d.
Compared to the anodization of the flat Al foil, the porous alumina growth on the hemisphere curved surface could enlarge the whole surface area. From the viewpoint of geometry, the surface area is 2πr 2 in a hemisphere and πr 2 on a circle plane. That is, it is about two times the surface area by the anodization of Al foil compared with the hemisphere curved surface. It is very helpful for photocatalyst or sensor applications. By filling the nanopore with TiO2 materials like titanium dioxide , a large surface area can enhance photocatalyst performance. On the other hand, the particular branch structure of alumina pore channel can be used in fabricating Y-shaped carbon nanotubes .
The behavior of porous alumina on a hemisphere curved surface has been demonstrated and examined by an HPA process on low-purity Al foil at RT. The hemisphere curve is formed through the Joule heat caused by the impurity and isotropic heat conduction phenomenon. The growth of nanopore is found to move along the normal vector of a hemisphere curve. The impurity with high electric resistivity can generate much more Joule heat around the impurity location for accelerating the electrochemistry response. Moreover, the pore channel positioned at the curve center had several branching due to different directions of each pore and the unbalanced strongest electrical field at the edge of the pore at the bottom. As branching is formed in the central channel, the other pore growth is bending towards the outer area, while the conventional research results claim that the pore structures have been bended towards the concave center in a different way. The feature of branching and bending of pore structures on the high-curvature hemisphere curve is induced by electric field rather than the large interpore distance in the conventional low-curvature cavity. Such a process for enhancing the AAO surface area is cost-saving for potential photocatalyst or sensor applications or Y-shaped carbon nanotube fabrications in the future.
This work is partially sponsored by the National Science Council under contract number NSC99-2221-E-006-032-MY3. We also would like to thank the Center for Micro/Nano Science and Technology of the National Cheng Kung University, National Nano Device Laboratories (NDL), and National Center for High-Performance Computing (NCHC) for the access of the process and analysis equipment.
- Diggle JW, Downie TC, Goulding CW: Anodic oxide films on aluminum. Chem Rev 1969, 69: 365–405. 10.1021/cr60259a005View ArticleGoogle Scholar
- Masuda H, Fukuda F: Ordered metal nanohole arrays made by a two-step replication of honeycomb structures of anodic alumina. Science 1995, 268: 1466–1468. 10.1126/science.268.5216.1466View ArticleGoogle Scholar
- Gleiter H: Nanostructured materials: basic concepts and microstructure. Acta Materialia 2000, 48: 1–29. 10.1016/S1359-6454(99)00285-2View ArticleGoogle Scholar
- Kawakami S, Kawashima T, Sato T: Mechanism of shape formation of three-dimensional periodic nanostructures by bias sputtering. Appl Phys Lett 1999, 74: 463–465. 10.1063/1.123037View ArticleGoogle Scholar
- Zang KY, Wang YD, Liu HF, Chua SJ: Structural and optical properties of InGaN/GaN multiple quantum wells grown on nano-air-bridged GaN template. Appl Phys Lett 2006, 89: 171921. 10.1063/1.2372686View ArticleGoogle Scholar
- Mizeikis V, Mikulskas I Tomasiunas R, Juodkazis S, Matsuo S, Misawa H: Optical characteristics of two-dimensional photonic crystals in anodic aluminum oxide films. Jpn J Appl Phys 2004, 43: 3643–3647. 10.1143/JJAP.43.3643View ArticleGoogle Scholar
- Wang YD, Zang KY, Chua SJ, Tripathy S, Chen P, Fonstad CG: Nanoair-bridged lateral overgrowth of GaN on ordered nanoporous GaN template. Appl Phys Lett 2005, 87: 251915. 10.1063/1.2147716View ArticleGoogle Scholar
- Nahar PK: Study of the performance degradation of thin film aluminum oxide sensor at high humidity. Sens Actuators B 2000, 63: 49–54. 10.1016/S0925-4005(99)00511-0View ArticleGoogle Scholar
- Zhang Z, Shimizu T, Senz S, Gosele U: Ordered high-density Si  nanowire arrays epitaxially grown by bottom imprint method. Adv Mater 2009, 21: 2824–2828. 10.1002/adma.200802156View ArticleGoogle Scholar
- Shelimov KB, Davydov DN, Moskovits M: Template-grown high-density nanocapacitor arrays. Appl Phys Lett 2000, 77: 1722–1724. 10.1063/1.1290598View ArticleGoogle Scholar
- Lee W, Schwirn K, Steinhart M, Pippel E, Scholz R, Gosele U: Structural engineering of nanoporous anodic aluminium oxide by pulse anodization of aluminium. Nat Nanotechnol 2008, 3: 234–239. 10.1038/nnano.2008.54View ArticleGoogle Scholar
- Hu GF, Zhang HM, Di WW, Zhao TT: Study on wet etching of AAO template. Appl Phys Res 2009, 1: 78–82.View ArticleGoogle Scholar
- Ye JM, Yin QM, Zhou YL: Superhydrophilicity of anodic aluminum oxide films: from "honeycomb" to "bird's nest". Thin Solid Films 2009, 517: 6012–6015. 10.1016/j.tsf.2009.04.042View ArticleGoogle Scholar
- Yin A, Guico RS, Xu J: Fabrication of anodic aluminium oxide templates on curved surfaces. Nanotechnology 2007, 18: 035304. 10.1088/0957-4484/18/3/035304View ArticleGoogle Scholar
- Chung CK, Zhou RX, Liu TY, Chang WT: Hybrid pulse anodization for the fabrication of porous anodic alumina films from commercial purity (99%) aluminum at room temperature. Nanotechnology 2009, 20: 055301. 10.1088/0957-4484/20/5/055301View ArticleGoogle Scholar
- Chung CK, Chang WT, Liao MW, Chang HC: Effect of pulse voltage and aluminum purity on the characteristics of anodic aluminum oxide using hybrid pulse anodization at room temperature. Thin Solid Films 2011, 519: 4754–4758. 10.1016/j.tsf.2011.01.029View ArticleGoogle Scholar
- Chung CK, Chang WT, Liao MW, Chang HC, Lee CT: Fabrication of enhanced anodic alumina oxide performance at room temperatures using hybrid pulse anodization with effective cooling. Electrochimica Acta 2011, 56: 6489–6497. 10.1016/j.electacta.2011.04.122View ArticleGoogle Scholar
- Chu SZ, Wada K, Inoue S, Todoroki S: Synthesis and characterization of titania nanostructures on glass by anodization and sol-gel process. Chem Mater 2002, 14: 266. 10.1021/cm0105918View ArticleGoogle Scholar
- Zhu HH, Ci L, Xu C, Liang J, Wu D: Growth mechanism of Y-junction carbon nanotubes. Diamond Rel Mater 2002, 11: 1349. 10.1016/S0925-9635(01)00745-2View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.